DOI 10.1007/s10948-008-0440-y L E T T E R
Muon-Spin Rotation Study of the Ternary Noncentrosymmetric
P.S. Häfliger· R. Khasanov · R. Lortz · A. Petrovi´c · K. Togano· C. Baines · B. Graneli · H. Keller
Received: 10 December 2008 / Accepted: 15 December 2008 / Published online: 13 January 2009 © Springer Science+Business Media, LLC 2009
Abstract We investigated the superconducting state of the noncentrosymmetric superconductors Li2PdxPt3−xB with superconducting transition temperature Tc = 5.16(8) K (x= 2.25), 3.56(8) K (x = 1.5) and 2.60 K (x = 0) by means of muon-spin rotation (µSR) and specific heat experiments. The µSR relaxation rate σscwas found to be constant at low temperatures for all the compounds. Data taken at different magnetic fields show that the magnetic penetration depth λ is field-independent for Li2Pd2.25Pt0.75B and Li2Pt3B. The electronic contribution to the specific heat measured in Li2Pd1.5Pt1.5B and Li2Pt3B increases exponentially at the lowest temperatures. These features suggest that the whole family of Li2PdxPt3−xB comprises single-gap s-wave super-conductors across the entire doping regime.
Keywords Noncentrosymmetric superconductors· Magnetic penetration depth
P.S. Häfliger· B. Graneli · H. Keller
Physik-Institut der Universität Zürich, Winterthurerstrasse 190, 8057 Zürich, Switzerland
R. Khasanov ()· C. Baines
Laboratory for Muon-Spin Spectroscopy, Paul Scherrer Institute, CH-5232 Villigen PSI, Switzerland
R. Lortz· A. Petrovi´c
Département de Physique de la Matière Condensée de Genève, 24 quai Ernest-Ansermet, 1211 Geneva, Switzerland
National Institute for Materials Science, 1-2-1 Sengen, Tsukuba 305-0047, Japan
Superconductivity in systems without inversion symmetry has recently attracted considerable interest, see e.g. [1,2]. The basic pairing states for a superconductor can be gener-ally classified as spin-singlet and spin-triplet states. Cooper pairing in the spin-singlet channel is based on time-reversal symmetry (Anderson’s theorem) , whereas for spin-triplet pairing also the existence of an inversion center in the crys-tal lattice is necessary . However, the lack of an inversion center in the crystal lattice induces an antisymmetric spin– orbit coupling (ASOC) which is not destructive to special spin-triplet states as has been shown by Frigeri et al.  in the case of CePt3Si, for instance.
Lately the noncentrosymmetric superconductors Li2Pd3B and Li2Pt3B have been discovered [6–9]. This system presents an ideal playing field to study superconductivity without inversion symmetry since there is no sign of mag-netic order or strong electron correlation effects  such as was found in CePt3Si, for instance. A significant effort was put into identifying the superconducting state using various experimental methods. While measurements of the penetra-tion depth  and nuclear magnetic resonance (NMR) ex-periments  suggest the existence of spin-triplet states and nodes in the gap of Li2Pt3B, specific heat data in-dicate conventional behavior as expected for an isotropic single-gap s-wave superconductor in Li2Pd3B and Li2Pt3B compounds . Furthermore, our previous muon-spin ro-tation (µSR) and magnetization experiments on Li2Pd3B show no sign of an unconventional superconducting pairing state [12,13].
In order to shed light on this controversy, we have per-formed a systematic study of Li2PdxPt3−xB at different doping levels x choosing the bulk-sensitive transverse-field
muon-spin rotation (TF-µSR) technique. Therewith we in-vestigated the temperature and field dependence of the µSR relaxation rate σ in Li2PdxPt3−xB with x= 2.25, 1.5 and 0. In addition, we measured the low-temperature specific heat of Li2Pd1.5Pt1.5B and Li2Pt3B.
Li2PdxPt3−xB was prepared by two-step arc-melting  for various doping concentrations. Details of the sample prepa-ration can be found elsewhere . The field-cooled mag-netization of all the compounds was measured using a su-perconducting quantum interference device (SQUID) mag-netometer in fields ranging from 0.5 mT to 1.6 T at temper-atures between 1.75 and 10 K. Specific heat was measured from 6 down to 0.1 K.
TF-µSR experiments were performed at the π M3 beam line at the Paul Scherrer Institute, Villigen, Switzerland. The Li2PdxPt3−xB (x= 2.25, 1.5 and 0) samples were field-cooled from above Tcdown to 30 mK in fields of 0.1, 0.02 and 0.01 T. We performed temperature scans at low fields for all the samples. Field-dependent data up to 1.5 T were taken for Li2Pd2.25Pt0.75B and Li2Pt3B where each point includes a set of data at T > Tcand at 1 K after cooling in the field.
The µSR signal was recorded in the usual time-differen-tial way by counting positrons from decaying muons as a function of time. The field distribution P (B) is then ob-tained from the Fourier transform of the measured time spectra P (t). P (t) is fitted with a Gaussian line and an os-cillatory term for the signal originating from the sample as well as for the signal belonging to the sample holder (silver plate). Figure1 illustrates the P (t) and P (B) distributions inside the Li2Pt3B sample in the mixed state at 0.05 K after being field-cooled in a magnetic field of 0.01 T. The sec-ond moment of P (B) is related to the µSR relaxation rate σ which contains the superconducting component σsc as well as a contribution from the nuclear moments, σ2= σsc2+ σn2.
3 Results and Discussion
In extreme type-II superconductors such as Li2Pd3B (Ginz-burg–Landau parameter κ≈ 27 ), the magnetic field distribution P (B) is almost independent of the coherence length ξ . The magnetic penetration depth λ can then be calculated from the known value of σsc using Brandt’s formula describing the field variation in an ideal triangular vortex lattice :
= 4.83 × 104(1− h)1+ 1.211−√h3
λ−2[nm] (1) where h= H/Hc2, with Hc2the upper critical field. Details can be found elsewhere, see e.g. .
The magnetic field dependence of the second moment of σsc(1 K) for Li2Pd2.25Pt0.75B and Li2Pt3B is displayed in the middle and right panels of Fig. 2, respectively. For the sake of completeness we also show the field depen-dence of σsc(0) for Li2Pd3B  in the left panel. The data are taken at a fixed field at a temperature T > Tc, the sample is then field-cooled to 1 K in order to deter-mine σsc and σn unambiguously for each field. The in-sets illustrate the corresponding temperature dependence of the upper critical field Hc2 as obtained from magnetiza-tion (Li2Pd3B and Li2Pd2.25Pt0.75B) and specific heat mea-surements (Li2Pt3B). Clearly Hc2(T ) can be satisfactorily fitted with the model based on the Werthamer–Helfand– Hohenberg (WHH) theory , as demonstrated by the solid lines. The results for Hc2(0) are listed in Table 1. Hc2 is then inserted into (1) in order to fit σsc(H ) to the exper-imental data with λ as a fit parameter. The results are in excellent agreement with the experimental data (shown by solid lines) implying that λ is field-independent. The devia-tion at low fields (h≤ 0.003 in the case of Li2Pd2.25Pt0.75B) is expected since (1) is no longer valid at this region. In the case of Li2Pt3B the error bars are large due to the
Fig. 1 µSR time spectrum (left
panel) and magnetic field
distribution (right panel) of Li2Pt3B taken in μ0H= 0.01 T
below the superconducting transition temperature
Tc= 2.60 K (0.05 K). The lines
represent a Gaussian fit as explained in the text
Fig. 2 Field dependence of the µSR depolarization rate
σsc(T= 1 K) in Li2PdxPt3−xB
for x= 3 (left panel)  as well as x= 2.25 (middle panel) and 0 (right panel). The solid lines correspond to the results of a least-squares fitting procedure based on (1) as described in the text. In the insets the upper critical field Hc2vs. temperature T is shown with the solid lines corresponding to a fit based on the WHH model
Table 1 Summary of the normal state and superconducting parame-ters for Li2PdxPt3−xB obtained in the present study from µSR mea-surements. The meaning of the parameters is explained in the text
x Tc[K] μ0Hc2[T] λ(0) [nm] κ(0) Δ0[meV] 2Δ0/ kBTc
3 7.66(5)a 3.66(8)a 252(2)a 27(1)a 1.53(4) 4.4(2) 2.25 5.16(8) 3.35(9) 413(8) 42(1) 1.03(4) 4.4(3) 1.5 3.56(8) 2.27(8) – – 0.59(2) 3.7(2) 0 2.60(5) 1.42(6) 608(10) 40(1) 0.41(2) 3.4(3)
small value of the relaxation rate σsc. The resulting pene-tration depth λ(1 K) equals 413(8) nm and 608(10) nm for Li2Pd2.25Pt0.75B and Li2Pt3B, respectively, while we ob-tained λ(0)= 252(2) nm for Li2Pd3B , see Table1. The value of λ(0) for Li2Pd3B is in agreement with magnetiza-tion measurements performed by Badica et al. , whereas our results for λ(0) for Li2Pd2.25Pt0.75B and Li2Pt3B devi-ate from those in .
The superconducting coherence length ξ may be es-timated from Hc2 as ξ = [0/(2π Hc2)]0.5. We obtain ξ(0) = 9.5(2) nm (Li2Pd3B) , ξ(1 K)= 9.9(2) nm (Li2Pd2.25Pt0.75B) and 15.2(8) nm (Li2Pt3B). This results in a value for κ(0)= λ(0)/ξ(0) of 27(1) for Li2Pd3B  with κ(1 K)= 42(1) and 40(1) for Li2Pd2.25Pt0.75B and Li2Pt3B, respectively (see Table1). Since λ is constant at low temper-atures as will be shown later, we may set ξ(0)≈ ξ(1 K) as well as λ(0)≈ λ(1 K). The compounds in the present work are thus extreme type-II superconductors; µSR is therefore an appropriate tool for penetration depth studies.
We also measured the temperature dependence of the µSR signal in order to extract λ−2(T ) using (1). The re-sults are displayed in Fig. 3 for the entire doping series Li2PdxPt3−xB (x= 0, 1.5, 2.25 and 3 ). The second moment of P (B) increases with x, and λ−2(x) monotoni-cally grows in turn with increasing Pd content. We observe that λ−2(T ) saturates at low temperatures and becomes
T-independent for all the compounds. This indicates that the Fermi surface is fully gapped down to the lowest tempera-tures. Thus we applied a model for a BCS s-wave supercon-ductor in order to fit the data (see e.g. )
λ−2(0) λ−2(T )= 1 + 2 · ∞ 0 dεdf dE . (2)
Here. . . represents an angular average over the Fermi sur-face, f is the Fermi function and E= ε2+ |Δ|2 the to-tal energy with ε the single-particle energy measured from the Fermi surface. Since we have assumed an isotropic gap, i.e. s-wave symmetry, the superconducting gap Δ is k-independent, but only depends on temperature T such that Δ(T )= Δ0· tanh(a
Tc/T − 1) with a = 1.74 . The resulting gap values at zero temperature Δ0are listed in Ta-ble1. Over the whole temperature range (Tcdown to 30 mK) and in the whole doping range (0≤ x ≤ 3) λ−2is consistent with what is expected for an isotropic BCS superconduc-tor. However, the BCS fit to the Li2Pt3B data is not satis-factory. In Li2Pt3B a considerable spin-triplet contribution has previously been observed in [10,11], thus we assumed a mixture of spin-triplet states associated with a strong an-tisymmetric spin–orbit coupling resulting in two bands as presented in . Assuming the same set of parameters and a BCS-temperature dependence of the superconducting gaps (black dotted line in Fig.3d), λ−2(T )differs significantly from our results. If we assume that the gap with nodes is smeared out due to inhomogeneity of the sample, the re-sulting model calculations are in agreement with our exper-imental data, as illustrated by the solid black line in Fig.3d. At this point we cannot exclude the existence of spin-triplet states.
In order to clarify matters, the superconducting state was also investigated by an independent study of the spe-cific heat. Figure4illustrates the specific heat obtained for Li2Pd1.5Pt1.5B (left panel) and Li2Pt3B (right panel) in zero
Fig. 3 Temperature dependence of λ−2in Li2PdxPt3−xB for x= 3 at 0.02 T (black open
circles) and 0.5 T (black solid circles) (panel a), 2.25 (panel
b), 1.5 (panel c) and 0 (panel d) at 0.01 T. The solid lines correspond to a least-squares fit to the experimental data for a BCS single-gap s-wave superconductor based on (2) with the parameters given in the text. In panel d, the gray dashed and dotted lines correspond to a model based on a two-gap scenario where one and both bands become superconducting, respectively; see text for explanation. The inset of panel
b illustrates Tcas a function of
Pd doping x
Fig. 4 Specific heat of Li2Pd1.5Pt1.5B (left panel) and
Li2Pt3B (right panel)
Table 2 Summary of the normal state and
superconducting parameters for Li2PdxPt3−xB obtained in the
present study from specific heat measurements. The meaning of the parameters is explained in the text x Tc[K] μ0Hc2[T] γ ΔC/γ Tc Δ0 2Δ0/ kBTc [mJ/gat K2] [meV] 3 7.66(5)a 3.66(8)a 1.50(2)b 2.0(3)b 1.30(4)b 3.94(4)b 2.25 5.16(8) 3.35(9) – – – – 1.5 3.56(8) 2.27(8) 1.10(2) 1.28(3) 0.37(2) 3.3(2) 0 2.60(5) 1.42(6) 1.66(2) 1.75(2) 0.45(2) 4.0(2)
field. The electronic contribution Ce/T to the specific heat of Li2Pt3B, as obtained in a standard procedure by quench-ing superconductivity in a field of 4 T, shows an exponential increase at the lowest temperature. This is consistent with our µSR data and therefore implies that Li2Pt3B is a fully gapped superconductor. A fit using a standard single-gap s-wave BCS model gives an excellent result (see Fig. 4). We obtain a gap-to-Tc ratio of 2Δ0/ kBTc= 4.0(2) which
is slightly larger than the µSR value but still in reasonable agreement. A smaller value of 2Δ0/ kBTc= 3.3(2) is de-rived for Li2Pd1.5Pt1.5B (see Table 2). A particularity of Li2Pt3B is a rather large residual Sommerfeld coefficient γr.
A possible explanation is that within a two-gap scenario as presented by Yuan et al.  only one gap becomes super-conducting, while the gap with nodes is smeared out due to inhomogeneity of the sample. However, we have measured
another piece of the same large sample and we found a vari-ation of γr of approximately 30%, but the superconducting
contribution remains unchanged. This behavior is typical for macroscopic metallic inclusions which remain in the normal state. Details of the specific heat measurements will be pub-lished elsewhere.
Interestingly, results in the literature postulate several dif-ferent superconducting ground states for the Li2PdxPt3−xB family. In particular, previous work on Li2Pt3B deviates substantially from our conclusions. For instance, Yuan et al.  found a linear temperature dependence of the low-temperature penetration depth in Li2Pt3B by using a tunnel-diode based, self-inductive technique. The results were in-terpreted on the basis of a parity-mixed state with two Fermi surfaces induced by the lack of inversion symmetry coupled with a strong ASOC. The authors found that in Li2Pt3B one of the superconducting gaps changes sign due to the en-hanced ASOC, which leads to line nodes in the supercon-ducting gap and therefore explains the non-saturating pen-etration depth. None of our data—neither µSR nor specific heat—supports such a scenario. We believe that the differ-ence in the experimental data arises from the different exper-imental techniques. In  data are taken by using a surface sensitive technique with the magnetic field only penetrat-ing a distance λ below the surface (200–600 nm, see Ta-ble1). Muons, on the other hand, penetrate to much bigger distances (fraction of millimeters) and therefore allow us to study the magnetic penetration depth in the bulk. The spe-cific heat is also a bulk-sensitive technique. Bearing these in mind, the discrepancy between the results obtained in the present study and those reported in  can be explained by the difference between the bulk and the surface proper-ties of Li2PdxPt3−xB, in analogy with what was observed in conventional  and unconventional  superconduc-tors. We would also like to emphasize that our data are in excellent agreement with the specific heat data presented in . Takeya et al. found values for 2Δ0/ kBTc= 3.94(4) and 3.53 for Li2Pd3B and Li2Pt3B, respectively, which are in reasonable agreement with our results obtained from µSR measurements.
We will briefly comment on the results of Nishiyama et al.  obtained using the nuclear magnetic resonance (NMR) technique which is also bulk-sensitive. They deduce the existence of triplet states in Li2Pt3B from the Knight shift. However, it is not clear why they use a p-wave model to fit the data for the spin relaxation rate. Furthermore, they predict the behavior for an s-wave symmetry of the super-conducting gap in Li2Pt3B by using the value for the super-conducting gap of Li2Pd3B which is more than three times bigger, see Table 1. In addition, the absence of a Hebel– Slichter peak in the spin relaxation does not necessarily im-ply that the sample under investigation has an anisotropic gap.
In conclusion, we have performed muon-spin rotation, spe-cific heat and magnetization measurements on the ternary boride superconductor Li2PdxPt3−xB. The main results are: (i) the field dependence of the µSR relaxation rate is consis-tent with Brandt’s formula, (ii) the upper critical field Hc2 obeys the WHH model, (iii) the temperature dependence of λ−2and (iv) the specific heat data are consistent with what is expected for an s-wave BCS superconductor. The temper-ature dependence of λ−2of Li2Pt3B can also be explained by the existence of two bands induced by an ASOC where only the one without nodes contributes to superconductivity due to inhomogeneity of the sample. But specific heat data indicate the existence of metallic inclusions. All our mea-surements and analysis strongly point to a single isotropic superconducting gap. No signature of an exotic supercon-ducting order parameter was found. Thus we suggest that the whole family of Li2PdxPt3−xB is a standard BCS super-conductor with a single, isotropic gap.
Acknowledgements This work was partly performed at the Swiss Muon Source (SµS), Paul Scherrer Institute (PSI, Switzerland). We are grateful to N. Hayashi and M. Sigrist for helpful discussions as well as to H. Takeya for providing us the samples Li2PdxPt3−xB,
x= 3, 2.25, 1.5 and 0. This work was supported by the Swiss National
Science Foundation and the K. Alex Müller Foundation.
1. Hayashi, N., Wakabayashi, K., Frigeri, P.A., Sigrist, M.: Phys. Rev. B 73, 024504 (2006)
2. Bauer, E., Hilscher, G., Michor, H., Paul, Ch., Scheidt, E.W., Grib-anov, A., Seropegin, Yu., Nöel, H., Sigrist, M., Rogl, P.: Phys. Rev. Lett. 92, 027003 (2004)
3. Anderson, P.W.: J. Phys. Chem. Solids 11, 26 (1959) 4. Anderson, P.W.: Phys. Rev. B 30, 4000 (1984)
5. Frigeri, P.A., Agterberg, D.F., Koga, A., Sigrist, M.: Phys. Rev. Lett. 92, 097001 (2004)
6. Togano, K., Badica, P., Nakamori, Y., Orimo, S., Takeya, H., Hi-rata, K.: Phys. Rev. Lett. 93, 247004 (2004)
7. Takeya, H., Hirata, K., Yamaura, K., Togano, K., El Massalami, M., Rapp, R., Chaves, F.A., Ouladdiaf, B.: Phys. Rev. B 72, 104506 (2005)
8. Badica, P., Kondo, T., Kudo, T., Nakamori, Y., Orimo, S., Togano, K.: Appl. Phys. Lett. 85, 4433 (2004)
9. Badica, P., Kondo, T., Togano, K.: J. Phys. Soc. Jpn. 74, 1014 (2005)
10. Yuan, H.Q., Agterberg, D.F., Hayashi, N., Badica, P., Vaderwelde, D., Togano, K., Sigrist, M., Salamon, M.B.: Phys. Rev. Lett. 97, 017006 (2006)
11. Nishiyama, M., Inada, Y., Zheng, G.-G.: Phys. Rev. Lett. 98, 047002 (2007)
12. Khasanov, R., Landau, I.L., Baines, C., La Mattina, F., Maisuradze, A., Togano, K., Keller, H.: Phys. Rev. B 73, 214528 (2006)
13. Landau, I.L., Khasanov, R., Togano, K., Keller, H.: Physica C 451, 134 (2007)
15. Brandt, E.H.: Phys. Rev. B 68, 054506 (2003)
16. Werthamer, N.R., Helfand, E., Hohenberg, P.C.: Phys. Rev. 147, 295 (1966)
17. Kim, M.-S., Skinta, J.A., Lemberger, T.R., Kang, W.N., Kim, H.-J., Choi, E.-M., Lee, S.-I.: Phys. Rev. B 66, 064511 (2002) 18. Bonalde, I., Yanoff, B.D., Salamon, M.B., Van Harlingen, D.J.,
Chia, E.M.E., Mao, Z.Q., Maeno, Y.: Phys. Rev. Lett. 85, 4775 (2000)
19. Khasanov, R., Di Castro, D., Paderno, Yu., Filippov, V., Brütsch, R., Keller, H.: Phys. Rev. B 72, 224509 (2005)
20. Khasanov, R., Shengelaya, A., Bussmann-Holder, A., Karpinski, J., Keller, H., Müller, K.A.: J. Supercond. Nov. Magn. 21, 81 (2008)